#------------------------------------------------------------------------------
#$Date: 2019-11-02 05:22:54 +0200 (Sat, 02 Nov 2019) $
#$Revision: 220693 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/12/74/4127420.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4127420
loop_
_publ_author_name
'Weippert, Valentin'
'Haffner, Arthur'
'Stamatopoulos, Alexis'
'Johrendt, Dirk'
_publ_section_title
;
 Supertetrahedral Layers Based on GaAs or InAs.
;
_journal_issue                   28
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              11245
_journal_page_last               11252
_journal_paper_doi               10.1021/jacs.9b04712
_journal_volume                  141
_journal_year                    2019
_chemical_formula_sum            'As32 Eu15 Ga22'
_chemical_formula_weight         6210.68
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_audit_creation_method           SHELXL-2016/6
_cell_angle_alpha                90
_cell_angle_beta                 98.2370(10)
_cell_angle_gamma                90
_cell_formula_units_Z            6
_cell_length_a                   22.8204(7)
_cell_length_b                   22.8257(7)
_cell_length_c                   19.7972(6)
_cell_measurement_reflns_used    6597
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      49.358
_cell_measurement_theta_min      5.075
_cell_volume                     10205.8(5)
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker D8 Quest'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_unetI/netI     0.0328
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            9028
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        24.757
_diffrn_reflns_theta_max         24.757
_diffrn_reflns_theta_min         2.323
_exptl_absorpt_coefficient_mu    37.581
_exptl_absorpt_correction_T_max  0.258209
_exptl_absorpt_correction_T_min  0.138539
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.063
_exptl_crystal_description       plate
_exptl_crystal_F_000             16098
_exptl_crystal_size_max          0.057
_exptl_crystal_size_mid          0.049
_exptl_crystal_size_min          0.018
_refine_diff_density_max         4.783
_refine_diff_density_min         -4.542
_refine_diff_density_rms         0.505
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.085
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     478
_refine_ls_number_reflns         9028
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.085
_refine_ls_R_factor_all          0.0926
_refine_ls_R_factor_gt           0.0724
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0612P)²+2000.9712P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1573
_refine_ls_wR_factor_ref         0.1674
_reflns_Friedel_coverage         0.000
_reflns_number_gt                7162
_reflns_number_total             9028
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            ja9b04712_si_003.cif
_cod_data_source_block           shelx
_cod_database_code               4127420
_shelx_shelxl_version_number     2016/6
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.223
_shelx_estimated_absorpt_t_max   0.551
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Eu1 Eu 0.01088(5) 0.06487(5) 0.58035(6) 0.0097(3) Uani 1 1 d . . .
Eu2 Eu 0.13758(5) 0.05967(5) 0.07337(6) 0.0091(3) Uani 1 1 d . . .
Eu3 Eu 0.18102(5) 0.37823(5) 0.42681(6) 0.0089(3) Uani 1 1 d . . .
Eu4 Eu 0.26231(5) 0.18617(5) 0.07840(6) 0.0099(3) Uani 1 1 d . . .
Eu5 Eu 0.30452(5) 0.25098(5) 0.42016(6) 0.0097(3) Uani 1 1 d . . .
Eu6 Eu 0.31275(5) 0.03275(5) 0.23472(6) 0.0156(3) Uani 1 1 d . . .
Eu7 Eu 0.31436(5) 0.40551(6) 0.26504(6) 0.0164(3) Uani 1 1 d . . .
Eu8 Eu 0.38529(5) 0.31180(5) 0.07981(6) 0.0098(3) Uani 1 1 d . . .
Eu9 Eu 0.4278(2) 0.2800(3) 0.26860(15) 0.146(3) Uani 0.692(6) 1 d . . P
Eu10 Eu 0.4395(3) 0.1426(3) 0.23084(19) 0.170(4) Uani 0.558(6) 1 d . . P
Eu11 Eu 0.44588(5) 0.00202(5) 0.07754(6) 0.0101(3) Uani 1 1 d . . .
Eu12 Eu 0.57156(5) 0.12579(5) 0.08047(6) 0.0096(3) Uani 1 1 d . . .
Ga1 Ga 0.01693(10) 0.09572(11) 0.39127(12) 0.0081(5) Uani 1 1 d . . .
Ga2 Ga 0.01821(10) 0.34264(10) 0.39175(12) 0.0078(5) Uani 1 1 d . . .
Ga3 Ga 0.03606(10) 0.21906(11) 0.54164(13) 0.0093(5) Uani 1 1 d . . .
Ga4 Ga 0.10601(10) 0.21841(11) 0.10826(12) 0.0084(5) Uani 1 1 d . . .
Ga5 Ga 0.10730(11) 0.46499(11) 0.11128(12) 0.0096(5) Uani 1 1 d . . .
Ga6 Ga 0.12313(10) 0.34283(11) 0.24667(12) 0.0076(5) Uani 1 1 d . . .
Ga7 Ga 0.12465(10) 0.09515(11) 0.25355(12) 0.0081(5) Uani 1 1 d . . .
Ga8 Ga 0.14079(10) 0.21967(11) 0.39153(12) 0.0086(5) Uani 1 1 d . . .
Ga9 Ga 0.16071(10) 0.09368(11) 0.53496(12) 0.0093(5) Uani 1 1 d . . .
Ga10 Ga 0.22825(10) 0.34440(11) 0.11128(12) 0.0092(5) Uani 1 1 d . . .
Ga11 Ga 0.24616(10) 0.21891(10) 0.24973(12) 0.0065(5) Uani 1 1 d . . .
Ga12 Ga 0.26515(10) 0.09428(11) 0.38679(12) 0.0084(5) Uani 1 1 d . . .
Ga13 Ga 0.28598(11) 0.03132(11) 0.03346(13) 0.0102(5) Uani 1 1 d . . .
Ga14 Ga 0.35750(11) 0.47145(11) 0.11322(12) 0.0098(5) Uani 1 1 d . . .
Ga15 Ga 0.41180(10) 0.15684(11) 0.04033(13) 0.0094(5) Uani 1 1 d . . .
Ga16 Ga 0.000000 0.21920(15) 0.250000 0.0077(7) Uani 1 2 d S T P
Ga17 Ga 0.000000 0.46490(15) 0.250000 0.0069(7) Uani 1 2 d S T P
Ga18 Ga 0.000000 0.97244(15) 0.250000 0.0085(7) Uani 1 2 d S T P
As1 As 0.03340(9) 0.40630(10) 0.03268(11) 0.0063(4) Uani 1 1 d . . .
As2 As 0.03689(9) 0.15540(9) 0.03091(11) 0.0055(4) Uani 1 1 d . . .
As3 As 0.05215(9) 0.28033(10) 0.17769(11) 0.0071(5) Uani 1 1 d . . .
As4 As 0.05610(10) 0.03202(10) 0.17794(11) 0.0079(5) Uani 1 1 d . . .
As5 As 0.07028(9) 0.15782(10) 0.32180(11) 0.0059(5) Uani 1 1 d . . .
As6 As 0.07420(9) 0.40606(10) 0.32249(11) 0.0067(5) Uani 1 1 d . . .
As7 As 0.08720(9) 0.03030(10) 0.46436(11) 0.0072(5) Uani 1 1 d . . .
As8 As 0.09075(9) 0.28328(10) 0.46920(11) 0.0062(5) Uani 1 1 d . . .
As9 As 0.10859(10) 0.15556(10) 0.61271(12) 0.0097(5) Uani 1 1 d . . .
As10 As 0.15923(9) 0.53244(10) 0.03802(11) 0.0062(5) Uani 1 1 d . . .
As11 As 0.16060(9) 0.27955(10) 0.03297(11) 0.0075(5) Uani 1 1 d . . .
As12 As 0.17794(9) 0.15391(10) 0.17769(11) 0.0069(5) Uani 1 1 d . . .
As13 As 0.18094(9) 0.40859(9) 0.18579(11) 0.0066(5) Uani 1 1 d . . .
As14 As 0.19580(9) 0.28421(10) 0.32201(11) 0.0066(5) Uani 1 1 d . . .
As15 As 0.19832(9) 0.02954(10) 0.31324(11) 0.0076(5) Uani 1 1 d . . .
As16 As 0.21539(9) 0.15845(10) 0.46435(11) 0.0060(4) Uani 1 1 d . . .
As17 As 0.23328(10) 0.03094(10) 0.61092(11) 0.0088(5) Uani 1 1 d . . .
As18 As 0.28653(9) 0.40498(10) 0.03765(11) 0.0071(5) Uani 1 1 d . . .
As19 As 0.30323(10) 0.28323(10) 0.18349(12) 0.0114(5) Uani 1 1 d . . .
As20 As 0.32204(10) 0.15567(10) 0.31368(12) 0.0107(5) Uani 1 1 d . . .
As21 As 0.35721(10) 0.09293(10) 0.11168(11) 0.0087(5) Uani 1 1 d . . .
As22 As 0.42800(10) 0.40545(10) 0.18624(12) 0.0104(5) Uani 1 1 d . . .
As23 As 0.44479(10) 0.03070(10) 0.31629(12) 0.0103(5) Uani 1 1 d . . .
As24 As 0.48346(10) 0.21877(10) 0.12295(12) 0.0108(5) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
As4 Eu1 As9 100.99(7) 6_556 .
As4 Eu1 As22 85.00(7) 6_556 8_456
As9 Eu1 As22 102.07(7) . 8_456
As4 Eu1 As2 174.50(7) 6_556 2
As9 Eu1 As2 82.46(6) . 2
As22 Eu1 As2 98.55(6) 8_456 2
As4 Eu1 As7 80.72(6) 6_556 5_556
As9 Eu1 As7 175.57(7) . 5_556
As22 Eu1 As7 82.11(6) 8_456 5_556
As2 Eu1 As7 95.53(6) 2 5_556
As4 Eu1 As7 96.21(6) 6_556 .
As9 Eu1 As7 81.95(6) . .
As22 Eu1 As7 175.53(7) 8_456 .
As2 Eu1 As7 79.94(6) 2 .
As7 Eu1 As7 93.82(6) 5_556 .
As4 Eu1 Ga18 43.46(6) 6_556 5_566
As9 Eu1 Ga18 96.54(6) . 5_566
As22 Eu1 Ga18 43.13(5) 8_456 5_566
As2 Eu1 Ga18 140.87(7) 2 5_566
As7 Eu1 Ga18 87.52(6) 5_556 5_566
As7 Eu1 Ga18 138.91(6) . 5_566
As4 Eu1 Ga3 141.98(7) 6_556 .
As9 Eu1 Ga3 42.14(6) . .
As22 Eu1 Ga3 93.49(6) 8_456 .
As2 Eu1 Ga3 42.39(6) 2 .
As7 Eu1 Ga3 136.81(6) 5_556 .
As7 Eu1 Ga3 88.21(6) . .
Ga18 Eu1 Ga3 117.91(7) 5_566 .
As4 Eu1 Ga9 92.43(6) 6_556 .
As9 Eu1 Ga9 42.16(6) . .
As22 Eu1 Ga9 142.97(7) 8_456 .
As2 Eu1 Ga9 87.27(6) 2 .
As7 Eu1 Ga9 134.00(6) 5_556 .
As7 Eu1 Ga9 41.40(6) . .
Ga18 Eu1 Ga9 117.92(5) 5_566 .
Ga3 Eu1 Ga9 66.56(6) . .
As4 Eu1 Ga14 88.22(6) 6_556 8_456
As9 Eu1 Ga14 142.12(7) . 8_456
As22 Eu1 Ga14 41.66(6) 8_456 8_456
As2 Eu1 Ga14 91.65(6) 2 8_456
As7 Eu1 Ga14 41.63(6) 5_556 8_456
As7 Eu1 Ga14 133.97(7) . 8_456
Ga18 Eu1 Ga14 65.39(4) 5_566 8_456
Ga3 Eu1 Ga14 115.31(6) . 8_456
Ga9 Eu1 Ga14 175.37(6) . 8_456
As4 Eu1 Eu8 133.90(6) 6_556 8_456
As9 Eu1 Eu8 91.42(5) . 8_456
As22 Eu1 Eu8 48.92(5) 8_456 8_456
As2 Eu1 Eu8 49.69(4) 2 8_456
As7 Eu1 Eu8 90.26(5) 5_556 8_456
As7 Eu1 Eu8 129.62(5) . 8_456
Ga18 Eu1 Eu8 91.40(5) 5_566 8_456
Ga3 Eu1 Eu8 57.29(4) . 8_456
Ga9 Eu1 Eu8 123.80(5) . 8_456
Ga14 Eu1 Eu8 58.07(4) 8_456 8_456
As4 Eu1 Eu2 48.01(5) 6_556 6_556
As9 Eu1 Eu2 88.84(5) . 6_556
As22 Eu1 Eu2 133.01(6) 8_456 6_556
As2 Eu1 Eu2 128.32(5) 2 6_556
As7 Eu1 Eu2 89.34(5) 5_556 6_556
As7 Eu1 Eu2 48.38(4) . 6_556
Ga18 Eu1 Eu2 90.63(5) 5_566 6_556
Ga3 Eu1 Eu2 122.01(5) . 6_556
Ga9 Eu1 Eu2 55.45(4) . 6_556
Ga14 Eu1 Eu2 122.51(5) 8_456 6_556
Eu8 Eu1 Eu2 177.91(4) 8_456 6_556
As17 Eu2 As12 100.35(7) 6 .
As17 Eu2 As4 100.45(7) 6 .
As12 Eu2 As4 80.75(6) . .
As17 Eu2 As7 84.27(7) 6 6
As12 Eu2 As7 175.33(7) . 6
As4 Eu2 As7 97.78(7) . 6
As17 Eu2 As18 83.97(6) 6 7
As12 Eu2 As18 98.77(7) . 7
As4 Eu2 As18 175.58(7) . 7
As7 Eu2 As18 82.35(6) 6 7
As17 Eu2 As2 178.97(7) 6 .
As12 Eu2 As2 80.26(6) . .
As4 Eu2 As2 80.46(6) . .
As7 Eu2 As2 95.14(6) 6 .
As18 Eu2 As2 95.13(6) 7 .
As17 Eu2 Ga9 43.22(6) 6 6
As12 Eu2 Ga9 141.83(7) . 6
As4 Eu2 Ga9 93.66(6) . 6
As7 Eu2 Ga9 42.48(6) 6 6
As18 Eu2 Ga9 89.41(6) 7 6
As2 Eu2 Ga9 136.37(6) . 6
As17 Eu2 Ga13 43.16(6) 6 .
As12 Eu2 Ga13 94.16(6) . .
As4 Eu2 Ga13 142.07(7) . .
As7 Eu2 Ga13 89.71(6) 6 .
As18 Eu2 Ga13 42.28(6) 7 .
As2 Eu2 Ga13 136.06(6) . .
Ga9 Eu2 Ga13 67.45(6) 6 .
As17 Eu2 Ga7 93.85(6) 6 .
As12 Eu2 Ga7 41.30(6) . .
As4 Eu2 Ga7 41.42(6) . .
As7 Eu2 Ga7 138.25(6) 6 .
As18 Eu2 Ga7 139.09(6) 7 .
As2 Eu2 Ga7 87.15(6) . .
Ga9 Eu2 Ga7 116.43(6) 6 .
Ga13 Eu2 Ga7 116.84(6) . .
As17 Eu2 Eu4 90.08(5) 6 .
As12 Eu2 Eu4 48.16(5) . .
As4 Eu2 Eu4 128.91(6) . .
As7 Eu2 Eu4 133.14(5) 6 .
As18 Eu2 Eu4 50.79(5) 7 .
As2 Eu2 Eu4 89.73(5) . .
Ga9 Eu2 Eu4 124.71(5) 6 .
Ga13 Eu2 Eu4 57.29(5) . .
Ga7 Eu2 Eu4 88.46(5) . .
As17 Eu2 Eu1 90.31(5) 6 6
As12 Eu2 Eu1 128.32(5) . 6
As4 Eu2 Eu1 47.58(5) . 6
As7 Eu2 Eu1 50.40(5) 6 6
As18 Eu2 Eu1 132.75(6) 7 6
As2 Eu2 Eu1 89.94(5) . 6
Ga9 Eu2 Eu1 57.32(4) 6 6
Ga13 Eu2 Eu1 124.75(5) . 6
Ga7 Eu2 Eu1 88.00(5) . 6
Eu4 Eu2 Eu1 176.45(4) . 6
As17 Eu2 Eu8 131.81(6) 6 7
As12 Eu2 Eu8 89.45(5) . 7
As4 Eu2 Eu8 127.74(6) . 7
As7 Eu2 Eu8 87.97(5) 6 7
As18 Eu2 Eu8 47.84(5) 7 7
As2 Eu2 Eu8 47.29(4) . 7
Ga9 Eu2 Eu8 121.90(5) 6 7
Ga13 Eu2 Eu8 89.47(5) . 7
Ga7 Eu2 Eu8 121.54(5) . 7
Eu4 Eu2 Eu8 62.17(3) . 7
Eu1 Eu2 Eu8 119.81(4) 6 7
As17 Eu3 As6 100.03(7) 7_556 .
As17 Eu3 As14 100.20(7) 7_556 .
As6 Eu3 As14 80.77(6) . .
As17 Eu3 As16 84.26(6) 7_556 7_556
As6 Eu3 As16 175.66(7) . 7_556
As14 Eu3 As16 97.86(7) . 7_556
As17 Eu3 As10 84.21(6) 7_556 6_566
As6 Eu3 As10 98.71(6) . 6_566
As14 Eu3 As10 175.58(7) . 6_566
As16 Eu3 As10 82.34(6) 7_556 6_566
As17 Eu3 As8 179.02(7) 7_556 .
As6 Eu3 As8 80.48(6) . .
As14 Eu3 As8 80.70(6) . .
As16 Eu3 As8 95.25(6) 7_556 .
As10 Eu3 As8 94.88(6) 6_566 .
As17 Eu3 Ga13 43.25(6) 7_556 4
As6 Eu3 Ga13 93.86(6) . 4
As14 Eu3 Ga13 141.89(7) . 4
As16 Eu3 Ga13 89.74(6) 7_556 4
As10 Eu3 Ga13 42.44(6) 6_566 4
As8 Eu3 Ga13 135.94(6) . 4
As17 Eu3 Ga9 43.21(6) 7_556 7_556
As6 Eu3 Ga9 141.52(7) . 7_556
As14 Eu3 Ga9 93.59(6) . 7_556
As16 Eu3 Ga9 42.48(6) 7_556 7_556
As10 Eu3 Ga9 89.53(6) 6_566 7_556
As8 Eu3 Ga9 136.49(6) . 7_556
Ga13 Eu3 Ga9 67.49(6) 4 7_556
As17 Eu3 Ga6 93.78(6) 7_556 .
As6 Eu3 Ga6 41.33(6) . .
As14 Eu3 Ga6 41.29(6) . .
As16 Eu3 Ga6 138.22(6) 7_556 .
As10 Eu3 Ga6 139.14(6) 6_566 .
As8 Eu3 Ga6 87.16(6) . .
Ga13 Eu3 Ga6 116.82(6) 4 .
Ga9 Eu3 Ga6 116.38(6) 7_556 .
As17 Eu3 Eu11 90.13(5) 7_556 4
As6 Eu3 Eu11 48.23(5) . 4
As14 Eu3 Eu11 129.00(5) . 4
As16 Eu3 Eu11 132.99(6) 7_556 4
As10 Eu3 Eu11 50.65(5) 6_566 4
As8 Eu3 Eu11 89.59(5) . 4
Ga13 Eu3 Eu11 57.18(4) 4 4
Ga9 Eu3 Eu11 124.64(5) 7_556 4
Ga6 Eu3 Eu11 88.65(5) . 4
As17 Eu3 Eu5 90.34(5) 7_556 .
As6 Eu3 Eu5 128.49(6) . .
As14 Eu3 Eu5 47.72(5) . .
As16 Eu3 Eu5 50.31(5) 7_556 .
As10 Eu3 Eu5 132.64(5) 6_566 .
As8 Eu3 Eu5 90.00(5) . .
Ga13 Eu3 Eu5 124.81(5) 4 .
Ga9 Eu3 Eu5 57.34(4) 7_556 .
Ga6 Eu3 Eu5 88.07(5) . .
Eu11 Eu3 Eu5 176.71(4) 4 .
As17 Eu3 Eu12 131.88(6) 7_556 8_456
As6 Eu3 Eu12 89.68(5) . 8_456
As14 Eu3 Eu12 127.91(5) . 8_456
As16 Eu3 Eu12 87.93(5) 7_556 8_456
As10 Eu3 Eu12 47.67(5) 6_566 8_456
As8 Eu3 Eu12 47.21(4) . 8_456
Ga13 Eu3 Eu12 89.46(5) 4 8_456
Ga9 Eu3 Eu12 121.88(5) 7_556 8_456
Ga6 Eu3 Eu12 121.60(5) . 8_456
Eu11 Eu3 Eu12 62.10(3) 4 8_456
Eu5 Eu3 Eu12 119.65(4) . 8_456
As12 Eu4 As21 100.85(7) . .
As12 Eu4 As19 84.05(6) . .
As21 Eu4 As19 102.64(7) . .
As12 Eu4 As11 175.09(7) . 7
As21 Eu4 As11 82.65(6) . 7
As19 Eu4 As11 98.61(7) . 7
As12 Eu4 As18 96.89(6) . 7
As21 Eu4 As18 82.17(6) . 7
As19 Eu4 As18 174.87(7) . 7
As11 Eu4 As18 80.09(6) 7 7
As12 Eu4 As11 80.84(6) . .
As21 Eu4 As11 175.86(7) . .
As19 Eu4 As11 81.26(7) . .
As11 Eu4 As11 95.44(6) 7 .
As18 Eu4 As11 93.90(6) 7 .
As12 Eu4 Ga11 42.95(6) . .
As21 Eu4 Ga11 96.24(6) . .
As19 Eu4 Ga11 42.89(6) . .
As11 Eu4 Ga11 140.55(7) 7 .
As18 Eu4 Ga11 139.08(6) 7 .
As11 Eu4 Ga11 87.57(6) . .
As12 Eu4 Ga15 141.83(7) . .
As21 Eu4 Ga15 42.31(6) . .
As19 Eu4 Ga15 93.96(6) . .
As11 Eu4 Ga15 42.40(6) 7 .
As18 Eu4 Ga15 88.40(6) 7 .
As11 Eu4 Ga15 136.68(6) . .
Ga11 Eu4 Ga15 117.62(6) . .
As12 Eu4 Ga13 92.98(6) . .
As21 Eu4 Ga13 42.28(6) . .
As19 Eu4 Ga13 143.66(7) . .
As11 Eu4 Ga13 87.31(6) 7 .
As18 Eu4 Ga13 41.43(6) 7 .
As11 Eu4 Ga13 134.15(7) . .
Ga11 Eu4 Ga13 118.03(6) . .
Ga15 Eu4 Ga13 66.64(6) . .
As12 Eu4 Eu8 132.68(6) . .
As21 Eu4 Eu8 91.32(5) . .
As19 Eu4 Eu8 48.62(5) . .
As11 Eu4 Eu8 50.12(5) 7 .
As18 Eu4 Eu8 130.19(5) 7 .
As11 Eu4 Eu8 90.25(5) . .
Ga11 Eu4 Eu8 90.64(5) . .
Ga15 Eu4 Eu8 57.32(4) . .
Ga13 Eu4 Eu8 123.93(5) . .
As12 Eu4 Eu2 48.16(5) . .
As21 Eu4 Eu2 89.00(5) . .
As19 Eu4 Eu2 132.21(5) . .
As11 Eu4 Eu2 129.00(6) 7 .
As18 Eu4 Eu2 48.91(4) 7 .
As11 Eu4 Eu2 89.37(5) . .
Ga11 Eu4 Eu2 90.27(5) . .
Ga15 Eu4 Eu2 122.53(5) . .
Ga13 Eu4 Eu2 55.89(4) . .
Eu8 Eu4 Eu2 178.99(4) . .
As12 Eu4 Eu4 127.75(6) . 7
As21 Eu4 Eu4 130.99(6) . 7
As19 Eu4 Eu4 89.76(6) . 7
As11 Eu4 Eu4 48.45(5) 7 7
As18 Eu4 Eu4 85.68(5) 7 7
As11 Eu4 Eu4 46.99(4) . 7
Ga11 Eu4 Eu4 122.37(6) . 7
Ga15 Eu4 Eu4 90.26(5) . 7
Ga13 Eu4 Eu4 119.28(6) . 7
Eu8 Eu4 Eu4 62.12(3) . 7
Eu2 Eu4 Eu4 117.00(4) . 7
As14 Eu5 As9 100.75(7) . 7_556
As14 Eu5 As20 84.99(7) . .
As9 Eu5 As20 101.25(7) 7_556 .
As14 Eu5 As8 175.05(7) . 7_556
As9 Eu5 As8 82.42(6) 7_556 7_556
As20 Eu5 As8 98.17(7) . 7_556
As14 Eu5 As16 80.97(6) . .
As9 Eu5 As16 175.98(7) 7_556 .
As20 Eu5 As16 82.48(7) . .
As8 Eu5 As16 95.62(6) 7_556 .
As14 Eu5 As16 96.38(6) . 7_556
As9 Eu5 As16 82.07(6) 7_556 7_556
As20 Eu5 As16 176.14(7) . 7_556
As8 Eu5 As16 80.23(6) 7_556 7_556
As16 Eu5 As16 94.15(6) . 7_556
As14 Eu5 Ga11 43.36(6) . .
As9 Eu5 Ga11 96.27(6) 7_556 .
As20 Eu5 Ga11 43.07(6) . .
As8 Eu5 Ga11 140.48(7) 7_556 .
As16 Eu5 Ga11 87.48(6) . .
As16 Eu5 Ga11 138.98(6) 7_556 .
As14 Eu5 Ga3 141.61(7) . 7_556
As9 Eu5 Ga3 42.05(6) 7_556 7_556
As20 Eu5 Ga3 92.88(6) . 7_556
As8 Eu5 Ga3 42.37(6) 7_556 7_556
As16 Eu5 Ga3 136.85(6) . 7_556
As16 Eu5 Ga3 88.28(6) 7_556 7_556
Ga11 Eu5 Ga3 117.61(6) . 7_556
As14 Eu5 Ga9 92.39(6) . 7_556
As9 Eu5 Ga9 42.18(6) 7_556 7_556
As20 Eu5 Ga9 142.20(7) . 7_556
As8 Eu5 Ga9 87.43(6) 7_556 7_556
As16 Eu5 Ga9 134.41(6) . 7_556
As16 Eu5 Ga9 41.48(6) 7_556 7_556
Ga11 Eu5 Ga9 117.78(6) . 7_556
Ga3 Eu5 Ga9 66.52(6) 7_556 7_556
As14 Eu5 Ga12 88.39(6) . .
As9 Eu5 Ga12 141.51(7) 7_556 .
As20 Eu5 Ga12 41.87(6) . .
As8 Eu5 Ga12 91.44(6) 7_556 .
As16 Eu5 Ga12 41.79(6) . .
As16 Eu5 Ga12 134.43(6) 7_556 .
Ga11 Eu5 Ga12 65.28(6) . .
Ga3 Eu5 Ga12 114.97(6) 7_556 .
Ga9 Eu5 Ga12 175.91(6) 7_556 .
As14 Eu5 Eu12 133.59(6) . 2_655
As9 Eu5 Eu12 90.99(5) 7_556 2_655
As20 Eu5 Eu12 48.61(5) . 2_655
As8 Eu5 Eu12 49.61(5) 7_556 2_655
As16 Eu5 Eu12 90.39(5) . 2_655
As16 Eu5 Eu12 129.83(5) 7_556 2_655
Ga11 Eu5 Eu12 91.08(5) . 2_655
Ga3 Eu5 Eu12 57.09(4) 7_556 2_655
Ga9 Eu5 Eu12 123.57(5) 7_556 2_655
Ga12 Eu5 Eu12 57.92(4) . 2_655
As14 Eu5 Eu3 48.06(5) . .
As9 Eu5 Eu3 88.97(5) 7_556 .
As20 Eu5 Eu3 133.05(6) . .
As8 Eu5 Eu3 128.71(5) 7_556 .
As16 Eu5 Eu3 89.53(5) . .
As16 Eu5 Eu3 48.48(4) 7_556 .
Ga11 Eu5 Eu3 90.61(5) . .
Ga3 Eu5 Eu3 122.11(5) 7_556 .
Ga9 Eu5 Eu3 55.60(4) 7_556 .
Ga12 Eu5 Eu3 122.79(5) . .
Eu12 Eu5 Eu3 178.29(4) 2_655 .
As21 Eu6 As17 79.13(6) . 6
As21 Eu6 As20 89.38(7) . .
As17 Eu6 As20 140.00(7) 6 .
As21 Eu6 As23 90.72(7) . .
As17 Eu6 As23 140.45(7) 6 .
As20 Eu6 As23 77.03(6) . .
As21 Eu6 As15 140.31(7) . .
As17 Eu6 As15 87.10(6) 6 .
As20 Eu6 As15 77.67(6) . .
As23 Eu6 As15 121.59(7) . .
As21 Eu6 As13 140.87(7) . 4_545
As17 Eu6 As13 87.43(6) 6 4_545
As20 Eu6 As13 122.32(7) . 4_545
As23 Eu6 As13 76.66(6) . 4_545
As15 Eu6 As13 74.24(6) . 4_545
As21 Eu6 Ga12 130.78(7) . .
As17 Eu6 Ga12 127.63(7) 6 .
As20 Eu6 Ga12 42.49(6) . .
As23 Eu6 Ga12 87.67(6) . .
As15 Eu6 Ga12 41.35(6) . .
As13 Eu6 Ga12 86.17(6) 4_545 .
As21 Eu6 Ga5 131.51(7) . 4_545
As17 Eu6 Ga5 127.49(7) 6 4_545
As20 Eu6 Ga5 88.48(6) . 4_545
As23 Eu6 Ga5 41.86(6) . 4_545
As15 Eu6 Ga5 86.01(6) . 4_545
As13 Eu6 Ga5 40.81(6) 4_545 4_545
Ga12 Eu6 Ga5 69.23(6) . 4_545
As21 Eu6 Eu10 50.24(7) . .
As17 Eu6 Eu10 129.12(8) 6 .
As20 Eu6 Eu10 55.96(13) . .
As23 Eu6 Eu10 50.45(12) . .
As15 Eu6 Eu10 133.57(13) . .
As13 Eu6 Eu10 126.95(13) 4_545 .
Ga12 Eu6 Eu10 94.58(11) . .
Ga5 Eu6 Eu10 90.32(10) 4_545 .
As21 Eu6 Eu7 128.82(6) . 4_545
As17 Eu6 Eu7 49.69(5) 6 4_545
As20 Eu6 Eu7 128.05(6) . 4_545
As23 Eu6 Eu7 127.00(6) . 4_545
As15 Eu6 Eu7 50.39(5) . 4_545
As13 Eu6 Eu7 50.35(5) 4_545 4_545
Ga12 Eu6 Eu7 88.70(5) . 4_545
Ga5 Eu6 Eu7 88.17(5) 4_545 4_545
Eu10 Eu6 Eu7 175.65(15) . 4_545
As9 Eu7 As17 79.69(7) 7_556 7_556
As9 Eu7 As22 88.39(7) 7_556 .
As17 Eu7 As22 139.95(7) 7_556 .
As9 Eu7 As19 89.82(7) 7_556 .
As17 Eu7 As19 140.67(7) 7_556 .
As22 Eu7 As19 76.53(6) . .
As9 Eu7 As13 141.14(7) 7_556 .
As17 Eu7 As13 87.83(6) 7_556 .
As22 Eu7 As13 122.42(7) . .
As19 Eu7 As13 76.89(6) . .
As9 Eu7 As15 140.38(7) 7_556 4
As17 Eu7 As15 87.33(6) 7_556 4
As22 Eu7 As15 77.87(6) . 4
As19 Eu7 As15 121.75(7) . 4
As13 Eu7 As15 74.50(6) . 4
As9 Eu7 Ga14 129.90(7) 7_556 .
As17 Eu7 Ga14 128.02(7) 7_556 .
As22 Eu7 Ga14 42.50(6) . .
As19 Eu7 Ga14 87.44(6) . .
As13 Eu7 Ga14 86.39(6) . .
As15 Eu7 Ga14 41.55(6) 4 .
As9 Eu7 Ga10 130.81(7) 7_556 .
As17 Eu7 Ga10 128.00(7) 7_556 .
As22 Eu7 Ga10 88.31(6) . .
As19 Eu7 Ga10 41.96(6) . .
As13 Eu7 Ga10 40.93(6) . .
As15 Eu7 Ga10 86.23(6) 4 .
Ga14 Eu7 Ga10 69.21(6) . .
As9 Eu7 Eu9 49.41(6) 7_556 .
As17 Eu7 Eu9 128.96(7) 7_556 .
As22 Eu7 Eu9 54.67(10) . .
As19 Eu7 Eu9 50.87(10) . .
As13 Eu7 Eu9 127.65(11) . .
As15 Eu7 Eu9 132.52(11) 4 .
Ga14 Eu7 Eu9 93.57(9) . .
Ga10 Eu7 Eu9 90.64(9) . .
As9 Eu7 Eu6 129.57(6) 7_556 4
As17 Eu7 Eu6 49.88(5) 7_556 4
As22 Eu7 Eu6 128.36(6) . 4
As19 Eu7 Eu6 127.56(6) . 4
As13 Eu7 Eu6 50.66(5) . 4
As15 Eu7 Eu6 50.49(5) 4 4
Ga14 Eu7 Eu6 89.02(5) . 4
Ga10 Eu7 Eu6 88.58(5) . 4
Eu9 Eu7 Eu6 176.83(11) . 4
As19 Eu8 As22 81.45(7) . .
As19 Eu8 As2 176.76(7) . 7
As22 Eu8 As2 99.19(7) . 7
As19 Eu8 As24 99.03(7) . .
As22 Eu8 As24 98.14(7) . .
As2 Eu8 As24 84.05(6) 7 .
As19 Eu8 As11 99.41(7) . 7
As22 Eu8 As11 177.57(7) . 7
As2 Eu8 As11 79.83(6) 7 7
As24 Eu8 As11 83.99(6) . 7
As19 Eu8 As18 80.55(7) . .
As22 Eu8 As18 81.65(7) . .
As2 Eu8 As18 96.37(6) 7 .
As24 Eu8 As18 179.56(7) . .
As11 Eu8 As18 96.22(6) 7 .
As19 Eu8 Ga15 94.18(6) . .
As22 Eu8 Ga15 140.29(7) . .
As2 Eu8 Ga15 87.36(6) 7 .
As24 Eu8 Ga15 43.26(6) . .
As11 Eu8 Ga15 42.04(6) 7 .
As18 Eu8 Ga15 136.86(7) . .
As19 Eu8 Ga3 141.15(7) . 8
As22 Eu8 Ga3 93.43(6) . 8
As2 Eu8 Ga3 42.08(6) 7 8
As24 Eu8 Ga3 43.29(6) . 8
As11 Eu8 Ga3 87.32(6) 7 8
As18 Eu8 Ga3 137.09(7) . 8
Ga15 Eu8 Ga3 65.69(6) . 8
As19 Eu8 Eu9 52.38(10) . .
As22 Eu8 Eu9 56.24(11) . .
As2 Eu8 Eu9 130.55(11) 7 .
As24 Eu8 Eu9 61.78(7) . .
As11 Eu8 Eu9 126.05(11) 7 .
As18 Eu8 Eu9 117.80(7) . .
Ga15 Eu8 Eu9 89.92(9) . .
Ga3 Eu8 Eu9 92.90(8) 8 .
As19 Eu8 Eu4 49.70(5) . .
As22 Eu8 Eu4 131.13(6) . .
As2 Eu8 Eu4 129.66(5) 7 .
As24 Eu8 Eu4 89.40(5) . .
As11 Eu8 Eu4 49.84(4) 7 .
As18 Eu8 Eu4 90.44(5) . .
Ga15 Eu8 Eu4 56.56(4) . .
Ga3 Eu8 Eu4 122.25(5) 8 .
Eu9 Eu8 Eu4 87.14(12) . .
As19 Eu8 Eu1 131.05(6) . 8
As22 Eu8 Eu1 49.61(5) . 8
As2 Eu8 Eu1 49.65(5) 7 8
As24 Eu8 Eu1 89.55(5) . 8
As11 Eu8 Eu1 129.48(5) 7 8
As18 Eu8 Eu1 90.62(5) . 8
Ga15 Eu8 Eu1 122.26(5) . 8
Ga3 Eu8 Eu1 56.57(4) 8 8
Eu9 Eu8 Eu1 92.85(12) . 8
Eu4 Eu8 Eu1 178.82(4) . 8
As19 Eu8 Eu2 127.78(6) . 7
As22 Eu8 Eu2 90.20(5) . 7
As2 Eu8 Eu2 49.14(5) 7 7
As24 Eu8 Eu2 133.19(6) . 7
As11 Eu8 Eu2 87.48(5) 7 7
As18 Eu8 Eu2 47.23(4) . 7
Ga15 Eu8 Eu2 121.60(5) . 7
Ga3 Eu8 Eu2 90.49(5) 8 7
Eu9 Eu8 Eu2 146.41(10) . 7
Eu4 Eu8 Eu2 118.71(4) . 7
Eu1 Eu8 Eu2 61.76(3) 8 7
As9 Eu9 As24 84.49(10) 7_556 2_655
As9 Eu9 As19 94.52(12) 7_556 .
As24 Eu9 As19 148.8(3) 2_655 .
As9 Eu9 Eu10 134.3(2) 7_556 .
As24 Eu9 Eu10 69.70(14) 2_655 .
As19 Eu9 Eu10 89.8(2) . .
As9 Eu9 As22 88.94(14) 7_556 .
As24 Eu9 As22 134.0(2) 2_655 .
As19 Eu9 As22 77.04(9) . .
Eu10 Eu9 As22 136.06(12) . .
As9 Eu9 Eu9 123.04(18) 7_556 2_655
As24 Eu9 Eu9 66.31(15) 2_655 2_655
As19 Eu9 Eu9 135.23(15) . 2_655
Eu10 Eu9 Eu9 80.76(16) . 2_655
As22 Eu9 Eu9 80.04(9) . 2_655
As9 Eu9 As24 172.5(3) 7_556 .
As24 Eu9 As24 96.37(10) 2_655 .
As19 Eu9 As24 88.57(10) . .
Eu10 Eu9 As24 52.35(10) . .
As22 Eu9 As24 85.15(11) . .
Eu9 Eu9 As24 51.39(10) 2_655 .
As9 Eu9 Ga3 41.53(7) 7_556 7_556
As24 Eu9 Ga3 43.06(7) 2_655 7_556
As19 Eu9 Ga3 127.02(16) . 7_556
Eu10 Eu9 Ga3 102.95(14) . 7_556
As22 Eu9 Ga3 118.53(17) . 7_556
Eu9 Eu9 Ga3 97.71(15) 2_655 7_556
As24 Eu9 Ga3 139.27(11) . 7_556
As9 Eu9 Eu8 128.26(11) 7_556 .
As24 Eu9 Eu8 145.74(12) 2_655 .
As19 Eu9 Eu8 51.17(6) . .
Eu10 Eu9 Eu8 88.62(12) . .
As22 Eu9 Eu8 50.56(7) . .
Eu9 Eu9 Eu8 84.71(11) 2_655 .
As24 Eu9 Eu8 49.79(6) . .
Ga3 Eu9 Eu8 168.41(16) 7_556 .
As9 Eu9 Eu7 52.19(7) 7_556 .
As24 Eu9 Eu7 136.48(11) 2_655 .
As19 Eu9 Eu7 53.80(7) . .
Eu10 Eu9 Eu7 142.3(2) . .
As22 Eu9 Eu7 52.67(7) . .
Eu9 Eu9 Eu7 130.57(11) 2_655 .
As24 Eu9 Eu7 125.98(9) . .
Ga3 Eu9 Eu7 93.72(8) 7_556 .
Eu8 Eu9 Eu7 76.32(6) . .
As9 Eu9 Eu10 128.57(11) 7_556 2_655
As24 Eu9 Eu10 44.12(8) 2_655 2_655
As19 Eu9 Eu10 127.08(19) . 2_655
Eu10 Eu9 Eu10 39.2(2) . 2_655
As22 Eu9 Eu10 125.21(19) . 2_655
Eu9 Eu9 Eu10 47.29(16) 2_655 2_655
As24 Eu9 Eu10 52.94(8) . 2_655
Ga3 Eu9 Eu10 87.05(8) 7_556 2_655
Eu8 Eu9 Eu10 102.70(9) . 2_655
Eu7 Eu9 Eu10 177.8(2) . 2_655
As9 Eu9 Eu5 43.02(9) 7_556 .
As24 Eu9 Eu5 82.98(10) 2_655 .
As19 Eu9 Eu5 75.50(12) . .
Eu10 Eu9 Eu5 95.30(18) . .
As22 Eu9 Eu5 120.58(9) . .
Eu9 Eu9 Eu5 148.56(13) 2_655 .
As24 Eu9 Eu5 144.4(2) . .
Ga3 Eu9 Eu5 52.48(7) 7_556 .
Eu8 Eu9 Eu5 126.55(13) . .
Eu7 Eu9 Eu5 68.58(7) . .
Eu10 Eu9 Eu5 113.43(15) 2_655 .
Eu10 Eu10 As21 134.6(3) 2_655 .
Eu10 Eu10 As24 77.0(2) 2_655 .
As21 Eu10 As24 84.06(11) . .
Eu10 Eu10 As23 83.65(13) 2_655 .
As21 Eu10 As23 95.11(15) . .
As24 Eu10 As23 151.4(4) . .
Eu10 Eu10 Eu9 92.80(15) 2_655 .
As21 Eu10 Eu9 118.7(3) . .
As24 Eu10 Eu9 69.80(16) . .
As23 Eu10 Eu9 132.72(17) . .
Eu10 Eu10 As20 134.9(2) 2_655 .
As21 Eu10 As20 87.92(17) . .
As24 Eu10 As20 131.5(3) . .
As23 Eu10 As20 76.94(10) . .
Eu9 Eu10 As20 72.7(2) . .
Eu10 Eu10 As24 54.97(13) 2_655 2_655
As21 Eu10 As24 169.9(4) . 2_655
As24 Eu10 As24 96.71(12) . 2_655
As23 Eu10 As24 89.01(12) . 2_655
Eu9 Eu10 As24 52.87(11) . 2_655
As20 Eu10 As24 84.06(15) . 2_655
Eu10 Eu10 Ga15 107.2(3) 2_655 .
As21 Eu10 Ga15 41.37(7) . .
As24 Eu10 Ga15 42.86(7) . .
As23 Eu10 Ga15 128.1(2) . .
Eu9 Eu10 Ga15 98.09(17) . .
As20 Eu10 Ga15 116.9(2) . .
As24 Eu10 Ga15 139.28(13) 2_655 .
Eu10 Eu10 Eu12 86.25(16) 2_655 2_655
As21 Eu10 Eu12 127.49(13) . 2_655
As24 Eu10 Eu12 145.64(16) . 2_655
As23 Eu10 Eu12 51.26(7) . 2_655
Eu9 Eu10 Eu12 81.48(15) . 2_655
As20 Eu10 Eu12 49.99(8) . 2_655
As24 Eu10 Eu12 49.74(7) 2_655 2_655
Ga15 Eu10 Eu12 166.6(2) . 2_655
Eu10 Eu10 Eu6 136.28(13) 2_655 .
As21 Eu10 Eu6 51.94(7) . .
As24 Eu10 Eu6 135.61(14) . .
As23 Eu10 Eu6 54.04(8) . .
Eu9 Eu10 Eu6 122.7(3) . .
As20 Eu10 Eu6 52.40(8) . .
As24 Eu10 Eu6 125.48(12) 2_655 .
Ga15 Eu10 Eu6 93.30(10) . .
Eu12 Eu10 Eu6 75.97(7) 2_655 .
Eu10 Eu10 Eu9 48.03(17) 2_655 2_655
As21 Eu10 Eu9 128.81(12) . 2_655
As24 Eu10 Eu9 44.76(8) . 2_655
As23 Eu10 Eu9 128.9(2) . 2_655
Eu9 Eu10 Eu9 52.0(2) . 2_655
As20 Eu10 Eu9 122.6(2) . 2_655
As24 Eu10 Eu9 52.65(7) 2_655 2_655
Ga15 Eu10 Eu9 87.56(9) . 2_655
Eu12 Eu10 Eu9 102.38(10) 2_655 2_655
Eu6 Eu10 Eu9 174.6(3) . 2_655
Eu10 Eu10 Eu11 93.37(19) 2_655 .
As21 Eu10 Eu11 43.17(11) . .
As24 Eu10 Eu11 83.47(13) . .
As23 Eu10 Eu11 76.78(16) . .
Eu9 Eu10 Eu11 150.39(14) . .
As20 Eu10 Eu11 120.41(11) . .
As24 Eu10 Eu11 146.9(3) 2_655 .
Ga15 Eu10 Eu11 52.50(8) . .
Eu12 Eu10 Eu11 127.81(17) 2_655 .
Eu6 Eu10 Eu11 68.86(9) . .
Eu9 Eu10 Eu11 115.59(16) 2_655 .
As6 Eu11 As21 100.39(7) 4_545 .
As6 Eu11 As23 83.80(6) 4_545 2_655
As21 Eu11 As23 101.66(7) . 2_655
As6 Eu11 As1 176.01(7) 4_545 7
As21 Eu11 As1 82.51(6) . 7
As23 Eu11 As1 98.37(6) 2_655 7
As6 Eu11 As10 97.04(6) 4_545 7
As21 Eu11 As10 82.58(6) . 7
As23 Eu11 As10 175.48(7) 2_655 7
As1 Eu11 As10 80.54(6) 7 7
As6 Eu11 As1 81.10(6) 4_545 3_545
As21 Eu11 As1 176.34(7) . 3_545
As23 Eu11 As1 81.79(6) 2_655 3_545
As1 Eu11 As1 95.85(6) 7 3_545
As10 Eu11 As1 93.94(6) 7 3_545
As6 Eu11 Ga17 42.80(6) 4_545 3_545
As21 Eu11 Ga17 95.72(6) . 3_545
As23 Eu11 Ga17 42.61(5) 2_655 3_545
As1 Eu11 Ga17 140.02(7) 7 3_545
As10 Eu11 Ga17 139.10(6) 7 3_545
As1 Eu11 Ga17 87.64(6) 3_545 3_545
As6 Eu11 Ga15 141.21(7) 4_545 .
As21 Eu11 Ga15 42.19(6) . .
As23 Eu11 Ga15 93.42(6) 2_655 .
As1 Eu11 Ga15 42.27(6) 7 .
As10 Eu11 Ga15 88.70(6) 7 .
As1 Eu11 Ga15 136.95(6) 3_545 .
Ga17 Eu11 Ga15 117.11(7) 3_545 .
As6 Eu11 Ga13 92.78(6) 4_545 .
As21 Eu11 Ga13 42.43(6) . .
As23 Eu11 Ga13 142.79(7) 2_655 .
As1 Eu11 Ga13 87.52(6) 7 .
As10 Eu11 Ga13 41.69(6) 7 .
As1 Eu11 Ga13 134.41(7) 3_545 .
Ga17 Eu11 Ga13 117.72(5) 3_545 .
Ga15 Eu11 Ga13 66.67(6) . .
As6 Eu11 Ga5 87.55(6) 4_545 3_545
As21 Eu11 Ga5 141.55(7) . 3_545
As23 Eu11 Ga5 41.38(6) 2_655 3_545
As1 Eu11 Ga5 91.86(6) 7 3_545
As10 Eu11 Ga5 134.14(6) 7 3_545
As1 Eu11 Ga5 41.56(6) 3_545 3_545
Ga17 Eu11 Ga5 65.06(4) 3_545 3_545
Ga15 Eu11 Ga5 115.33(6) . 3_545
Ga13 Eu11 Ga5 175.83(6) . 3_545
As6 Eu11 Ga2 40.96(6) 4_545 4_545
As21 Eu11 Ga2 139.54(6) . 4_545
As23 Eu11 Ga2 87.65(6) 2_655 4_545
As1 Eu11 Ga2 135.52(6) 7 4_545
As10 Eu11 Ga2 90.09(6) 7 4_545
As1 Eu11 Ga2 41.18(5) 3_545 4_545
Ga17 Eu11 Ga2 64.99(7) 3_545 4_545
Ga15 Eu11 Ga2 177.67(6) . 4_545
Ga13 Eu11 Ga2 113.51(6) . 4_545
Ga5 Eu11 Ga2 64.32(5) 3_545 4_545
As6 Eu11 Eu12 132.28(6) 4_545 .
As21 Eu11 Eu12 90.76(5) . .
As23 Eu11 Eu12 48.49(5) 2_655 .
As1 Eu11 Eu12 49.98(5) 7 .
As10 Eu11 Eu12 130.52(5) 7 .
As1 Eu11 Eu12 90.66(5) 3_545 .
Ga17 Eu11 Eu12 90.27(5) 3_545 .
Ga15 Eu11 Eu12 57.08(4) . .
Ga13 Eu11 Eu12 123.74(5) . .
Ga5 Eu11 Eu12 58.30(4) 3_545 .
Ga2 Eu11 Eu12 122.63(5) 4_545 .
As23 Eu12 As20 81.95(7) 2_655 2_655
As23 Eu12 As8 176.39(7) 2_655 8
As20 Eu12 As8 99.14(7) 2_655 8
As23 Eu12 As10 80.72(7) 2_655 3_545
As20 Eu12 As10 81.93(7) 2_655 3_545
As8 Eu12 As10 96.00(6) 8 3_545
As23 Eu12 As24 99.12(7) 2_655 .
As20 Eu12 As24 98.22(7) 2_655 .
As8 Eu12 As24 84.16(6) 8 .
As10 Eu12 As24 179.76(7) 3_545 .
As23 Eu12 As1 99.17(7) 2_655 7
As20 Eu12 As1 177.36(7) 2_655 7
As8 Eu12 As1 79.60(6) 8 7
As10 Eu12 As1 95.87(6) 3_545 7
As24 Eu12 As1 83.99(6) . 7
As23 Eu12 Ga15 93.97(6) 2_655 .
As20 Eu12 Ga15 140.41(7) 2_655 .
As8 Eu12 Ga15 87.37(6) 8 .
As10 Eu12 Ga15 136.53(7) 3_545 .
As24 Eu12 Ga15 43.29(6) . .
As1 Eu12 Ga15 42.05(6) 7 .
As23 Eu12 Ga3 141.34(7) 2_655 8
As20 Eu12 Ga3 93.32(6) 2_655 8
As8 Eu12 Ga3 42.19(6) 8 8
As10 Eu12 Ga3 136.86(6) 3_545 8
As24 Eu12 Ga3 43.33(6) . 8
As1 Eu12 Ga3 87.29(6) 7 8
Ga15 Eu12 Ga3 65.78(6) . 8
As23 Eu12 Ga12 87.80(6) 2_655 2_655
As20 Eu12 Ga12 41.59(6) 2_655 2_655
As8 Eu12 Ga12 90.75(6) 8 2_655
As10 Eu12 Ga12 42.06(6) 3_545 2_655
As24 Eu12 Ga12 138.12(7) . 2_655
As1 Eu12 Ga12 135.91(6) 7 2_655
Ga15 Eu12 Ga12 177.51(6) . 2_655
Ga3 Eu12 Ga12 113.72(6) 8 2_655
As23 Eu12 Eu10 51.65(13) 2_655 2_655
As20 Eu12 Eu10 57.34(14) 2_655 2_655
As8 Eu12 Eu10 131.78(13) 8 2_655
As10 Eu12 Eu10 118.01(8) 3_545 2_655
As24 Eu12 Eu10 61.96(7) . 2_655
As1 Eu12 Eu10 125.21(14) 7 2_655
Ga15 Eu12 Eu10 89.39(11) . 2_655
Ga3 Eu12 Eu10 93.68(10) 8 2_655
Ga12 Eu12 Eu10 93.09(11) 2_655 2_655
As23 Eu12 Eu11 49.61(5) 2_655 .
As20 Eu12 Eu11 131.56(6) 2_655 .
As8 Eu12 Eu11 129.25(5) 8 .
As10 Eu12 Eu11 89.99(5) 3_545 .
As24 Eu12 Eu11 89.77(5) . .
As1 Eu12 Eu11 49.66(5) 7 .
Ga15 Eu12 Eu11 56.68(4) . .
Ga3 Eu12 Eu11 122.46(5) 8 .
Ga12 Eu12 Eu11 123.75(5) 2_655 .
Eu10 Eu12 Eu11 86.41(15) 2_655 .
As23 Eu12 Eu5 131.56(6) 2_655 2_655
As20 Eu12 Eu5 49.61(5) 2_655 2_655
As8 Eu12 Eu5 49.59(5) 8 2_655
As10 Eu12 Eu5 90.35(5) 3_545 2_655
As24 Eu12 Eu5 89.89(5) . 2_655
As1 Eu12 Eu5 129.19(5) 7 2_655
Ga15 Eu12 Eu5 122.47(5) . 2_655
Ga3 Eu12 Eu5 56.69(4) 8 2_655
Ga12 Eu12 Eu5 57.07(4) 2_655 2_655
Eu10 Eu12 Eu5 94.42(15) 2_655 2_655
Eu11 Eu12 Eu5 178.83(4) . 2_655
As5 Ga1 As4 112.53(12) . 2
As5 Ga1 As7 110.24(11) . .
As4 Ga1 As7 107.18(12) 2 .
As5 Ga1 As2 111.20(12) . 2
As4 Ga1 As2 108.03(11) 2 2
As7 Ga1 As2 107.44(11) . 2
As3 Ga2 As6 112.50(12) 2 .
As3 Ga2 As8 111.00(12) 2 .
As6 Ga2 As8 108.03(11) . .
As3 Ga2 As1 110.52(11) 2 2
As6 Ga2 As1 108.49(11) . 2
As8 Ga2 As1 106.06(11) . 2
As3 Ga2 Eu11 140.53(10) 2 4
As6 Ga2 Eu11 53.48(7) . 4
As8 Ga2 Eu11 108.47(9) . 4
As1 Ga2 Eu11 56.70(7) 2 4
As9 Ga3 As2 108.74(12) . 2
As9 Ga3 As8 108.67(11) . .
As2 Ga3 As8 110.87(12) 2 .
As9 Ga3 As24 107.52(12) . 8_456
As2 Ga3 As24 110.38(11) 2 8_456
As8 Ga3 As24 110.57(12) . 8_456
As9 Ga3 Eu1 55.39(7) . .
As2 Ga3 Eu1 56.70(7) 2 .
As8 Ga3 Eu1 141.96(10) . .
As24 Ga3 Eu1 107.34(9) 8_456 .
As9 Ga3 Eu5 55.34(7) . 7_556
As2 Ga3 Eu5 141.66(10) 2 7_556
As8 Ga3 Eu5 56.56(7) . 7_556
As24 Ga3 Eu5 107.83(9) 8_456 7_556
Eu1 Ga3 Eu5 108.43(7) . 7_556
As9 Ga3 Eu12 109.51(10) . 8_456
As2 Ga3 Eu12 141.74(10) 2 8_456
As8 Ga3 Eu12 56.30(7) . 8_456
As24 Ga3 Eu12 56.46(7) 8_456 8_456
Eu1 Ga3 Eu12 156.16(8) . 8_456
Eu5 Ga3 Eu12 66.23(5) 7_556 8_456
As9 Ga3 Eu8 109.74(9) . 8_456
As2 Ga3 Eu8 56.23(7) 2 8_456
As8 Ga3 Eu8 141.58(10) . 8_456
As24 Ga3 Eu8 56.27(7) 8_456 8_456
Eu1 Ga3 Eu8 66.14(5) . 8_456
Eu5 Ga3 Eu8 156.56(8) 7_556 8_456
Eu12 Ga3 Eu8 108.88(7) 8_456 8_456
As9 Ga3 Eu9 53.04(8) . 7_556
As2 Ga3 Eu9 127.91(15) 2 7_556
As8 Ga3 Eu9 121.14(15) . 7_556
As24 Ga3 Eu9 54.63(8) 8_456 7_556
Eu1 Ga3 Eu9 79.25(11) . 7_556
Eu5 Ga3 Eu9 73.87(11) 7_556 7_556
Eu12 Ga3 Eu9 76.96(11) 8_456 7_556
Eu8 Ga3 Eu9 82.70(11) 8_456 7_556
As3 Ga4 As12 112.47(12) . .
As3 Ga4 As2 110.92(11) . .
As12 Ga4 As2 108.04(12) . .
As3 Ga4 As11 110.41(12) . .
As12 Ga4 As11 108.43(11) . .
As2 Ga4 As11 106.34(11) . .
As13 Ga5 As23 108.29(12) . 4
As13 Ga5 As1 115.88(12) . .
As23 Ga5 As1 110.14(11) 4 .
As13 Ga5 As10 109.27(11) . .
As23 Ga5 As10 105.40(11) 4 .
As1 Ga5 As10 107.35(11) . .
As13 Ga5 Eu6 60.11(7) . 4
As23 Ga5 Eu6 59.25(8) 4 4
As1 Ga5 Eu6 161.97(10) . 4
As10 Ga5 Eu6 90.10(8) . 4
As13 Ga5 Eu11 143.32(10) . 3_455
As23 Ga5 Eu11 55.15(7) 4 3_455
As1 Ga5 Eu11 56.90(7) . 3_455
As10 Ga5 Eu11 106.90(9) . 3_455
Eu6 Ga5 Eu11 114.39(7) 4 3_455
As3 Ga6 As13 116.75(12) . .
As3 Ga6 As14 111.03(12) . .
As13 Ga6 As14 105.67(11) . .
As3 Ga6 As6 111.29(11) . .
As13 Ga6 As6 105.44(12) . .
As14 Ga6 As6 105.92(11) . .
As3 Ga6 Eu3 141.80(10) . .
As13 Ga6 Eu3 101.45(9) . .
As14 Ga6 Eu3 54.52(7) . .
As6 Ga6 Eu3 54.31(7) . .
As5 Ga7 As15 117.78(12) . .
As5 Ga7 As12 110.80(12) . .
As15 Ga7 As12 105.36(11) . .
As5 Ga7 As4 110.58(11) . .
As15 Ga7 As4 105.63(12) . .
As12 Ga7 As4 105.89(11) . .
As5 Ga7 Eu2 141.37(10) . .
As15 Ga7 Eu2 100.86(9) . .
As12 Ga7 Eu2 54.41(7) . .
As4 Ga7 Eu2 54.58(7) . .
As5 Ga8 As14 112.25(12) . .
As5 Ga8 As16 110.24(12) . .
As14 Ga8 As16 107.22(11) . .
As5 Ga8 As8 111.35(11) . .
As14 Ga8 As8 107.94(11) . .
As16 Ga8 As8 107.64(11) . .
As7 Ga9 As16 112.45(12) . .
As7 Ga9 As9 109.33(11) . .
As16 Ga9 As9 109.26(12) . .
As7 Ga9 As17 109.73(12) . .
As16 Ga9 As17 109.48(11) . .
As9 Ga9 As17 106.41(11) . .
As7 Ga9 Eu2 56.72(7) . 6_556
As16 Ga9 Eu2 142.05(10) . 6_556
As9 Ga9 Eu2 108.51(9) . 6_556
As17 Ga9 Eu2 55.28(7) . 6_556
As7 Ga9 Eu3 142.05(10) . 7_556
As16 Ga9 Eu3 56.62(7) . 7_556
As9 Ga9 Eu3 108.45(9) . 7_556
As17 Ga9 Eu3 55.10(7) . 7_556
Eu2 Ga9 Eu3 107.19(7) 6_556 7_556
As7 Ga9 Eu5 142.51(10) . 7_556
As16 Ga9 Eu5 57.32(7) . 7_556
As9 Ga9 Eu5 54.54(7) . 7_556
As17 Ga9 Eu5 107.48(9) . 7_556
Eu2 Ga9 Eu5 154.36(8) 6_556 7_556
Eu3 Ga9 Eu5 67.07(5) 7_556 7_556
As7 Ga9 Eu1 57.53(7) . .
As16 Ga9 Eu1 142.51(10) . .
As9 Ga9 Eu1 54.42(7) . .
As17 Ga9 Eu1 107.70(9) . .
Eu2 Ga9 Eu1 67.23(5) 6_556 .
Eu3 Ga9 Eu1 154.27(8) 7_556 .
Eu5 Ga9 Eu1 106.47(7) 7_556 .
As13 Ga10 As19 108.45(12) . .
As13 Ga10 As11 116.22(12) . .
As19 Ga10 As11 109.56(12) . .
As13 Ga10 As18 109.64(12) . .
As19 Ga10 As18 105.24(11) . .
As11 Ga10 As18 107.17(11) . .
As13 Ga10 Eu7 59.91(7) . .
As19 Ga10 Eu7 59.56(7) . .
As11 Ga10 Eu7 161.76(11) . .
As18 Ga10 Eu7 90.40(8) . .
As12 Ga11 As20 106.58(12) . .
As12 Ga11 As14 113.19(11) . .
As20 Ga11 As14 114.13(12) . .
As12 Ga11 As19 113.01(12) . .
As20 Ga11 As19 103.70(11) . .
As14 Ga11 As19 105.97(12) . .
As12 Ga11 Eu5 143.48(10) . .
As20 Ga11 Eu5 59.17(7) . .
As14 Ga11 Eu5 57.41(7) . .
As19 Ga11 Eu5 103.30(9) . .
As12 Ga11 Eu4 57.35(7) . .
As20 Ga11 Eu4 101.93(9) . .
As14 Ga11 Eu4 143.63(10) . .
As19 Ga11 Eu4 58.69(7) . .
Eu5 Ga11 Eu4 152.11(8) . .
As15 Ga12 As20 108.91(12) . .
As15 Ga12 As16 114.74(12) . .
As20 Ga12 As16 110.15(11) . .
As15 Ga12 As10 109.03(12) . 4_545
As20 Ga12 As10 106.53(11) . 4_545
As16 Ga12 As10 107.15(11) . 4_545
As15 Ga12 Eu6 60.51(7) . .
As20 Ga12 Eu6 59.71(7) . .
As16 Ga12 Eu6 161.80(11) . .
As10 Ga12 Eu6 90.69(8) 4_545 .
As15 Ga12 Eu5 143.06(10) . .
As20 Ga12 Eu5 55.51(7) . .
As16 Ga12 Eu5 56.59(7) . .
As10 Ga12 Eu5 107.66(9) 4_545 .
Eu6 Ga12 Eu5 115.21(7) . .
As15 Ga12 Eu12 137.36(10) . 2_655
As20 Ga12 Eu12 53.84(7) . 2_655
As16 Ga12 Eu12 107.89(9) . 2_655
As10 Ga12 Eu12 55.37(7) 4_545 2_655
Eu6 Ga12 Eu12 79.04(5) . 2_655
Eu5 Ga12 Eu12 65.01(5) . 2_655
As18 Ga13 As10 111.61(12) 7 7
As18 Ga13 As21 109.99(12) 7 .
As10 Ga13 As21 110.18(11) 7 .
As18 Ga13 As17 109.75(11) 7 6
As10 Ga13 As17 109.81(12) 7 6
As21 Ga13 As17 105.31(12) . 6
As18 Ga13 Eu3 141.79(11) 7 4_545
As10 Ga13 Eu3 57.02(7) 7 4_545
As21 Ga13 Eu3 108.01(9) . 4_545
As17 Ga13 Eu3 55.14(7) 6 4_545
As18 Ga13 Eu2 56.94(7) 7 .
As10 Ga13 Eu2 141.77(10) 7 .
As21 Ga13 Eu2 107.86(9) . .
As17 Ga13 Eu2 55.15(7) 6 .
Eu3 Ga13 Eu2 107.09(7) 4_545 .
As18 Ga13 Eu11 142.79(10) 7 .
As10 Ga13 Eu11 57.86(7) 7 .
As21 Ga13 Eu11 54.85(7) . .
As17 Ga13 Eu11 107.22(9) 6 .
Eu3 Ga13 Eu11 66.89(5) 4_545 .
Eu2 Ga13 Eu11 154.07(8) . .
As18 Ga13 Eu4 57.93(7) 7 .
As10 Ga13 Eu4 142.88(10) 7 .
As21 Ga13 Eu4 54.60(7) . .
As17 Ga13 Eu4 107.07(9) 6 .
Eu3 Ga13 Eu4 153.88(8) 4_545 .
Eu2 Ga13 Eu4 66.82(5) . .
Eu11 Ga13 Eu4 106.83(7) . .
As15 Ga14 As22 109.10(12) 4 .
As15 Ga14 As7 114.99(12) 4 4
As22 Ga14 As7 109.68(11) . 4
As15 Ga14 As18 109.28(11) 4 .
As22 Ga14 As18 106.42(11) . .
As7 Ga14 As18 107.01(11) 4 .
As15 Ga14 Eu7 60.44(8) 4 .
As22 Ga14 Eu7 59.99(7) . .
As7 Ga14 Eu7 161.75(11) 4 .
As18 Ga14 Eu7 90.82(9) . .
As15 Ga14 Eu1 143.12(10) 4 8
As22 Ga14 Eu1 55.12(7) . 8
As7 Ga14 Eu1 56.50(7) 4 8
As18 Ga14 Eu1 107.34(9) . 8
Eu7 Ga14 Eu1 115.10(7) . 8
As21 Ga15 As1 108.86(12) . 7
As21 Ga15 As11 109.10(11) . 7
As1 Ga15 As11 110.05(12) 7 7
As21 Ga15 As24 106.66(12) . .
As1 Ga15 As24 111.12(11) 7 .
As11 Ga15 As24 110.96(12) 7 .
As21 Ga15 Eu4 55.42(7) . .
As1 Ga15 Eu4 141.53(10) 7 .
As11 Ga15 Eu4 57.01(7) 7 .
As24 Ga15 Eu4 107.20(9) . .
As21 Ga15 Eu11 55.25(7) . .
As1 Ga15 Eu11 56.75(7) 7 .
As11 Ga15 Eu11 141.14(10) 7 .
As24 Ga15 Eu11 107.77(9) . .
Eu4 Ga15 Eu11 108.17(6) . .
As21 Ga15 Eu12 108.98(9) . .
As1 Ga15 Eu12 56.82(7) 7 .
As11 Ga15 Eu12 141.92(10) 7 .
As24 Ga15 Eu12 56.51(7) . .
Eu4 Ga15 Eu12 155.92(8) . .
Eu11 Ga15 Eu12 66.24(5) . .
As21 Ga15 Eu8 109.35(9) . .
As1 Ga15 Eu8 141.79(10) 7 .
As11 Ga15 Eu8 56.76(7) 7 .
As24 Ga15 Eu8 56.34(7) . .
Eu4 Ga15 Eu8 66.12(5) . .
Eu11 Ga15 Eu8 156.44(8) . .
Eu12 Ga15 Eu8 109.00(7) . .
As21 Ga15 Eu10 53.38(9) . .
As1 Ga15 Eu10 120.37(18) 7 .
As11 Ga15 Eu10 129.52(18) 7 .
As24 Ga15 Eu10 53.54(9) . .
Eu4 Ga15 Eu10 80.60(14) . .
Eu11 Ga15 Eu10 73.40(14) . .
Eu12 Ga15 Eu10 75.36(14) . .
Eu8 Ga15 Eu10 83.05(14) . .
As3 Ga16 As3 109.87(17) 2 .
As3 Ga16 As5 108.94(7) 2 .
As3 Ga16 As5 109.75(7) . .
As3 Ga16 As5 109.75(7) 2 2
As3 Ga16 As5 108.94(7) . 2
As5 Ga16 As5 109.57(17) . 2
As6 Ga17 As6 113.71(17) 2 .
As6 Ga17 As23 112.67(7) 2 4
As6 Ga17 As23 106.44(8) . 4
As6 Ga17 As23 106.44(8) 2 3_455
As6 Ga17 As23 112.67(7) . 3_455
As23 Ga17 As23 104.65(17) 4 3_455
As6 Ga17 Eu11 143.63(8) 2 4
As6 Ga17 Eu11 56.96(5) . 4
As23 Ga17 Eu11 103.45(9) 4 4
As23 Ga17 Eu11 58.45(6) 3_455 4
As6 Ga17 Eu11 56.96(5) 2 3_455
As6 Ga17 Eu11 143.63(8) . 3_455
As23 Ga17 Eu11 58.45(6) 4 3_455
As23 Ga17 Eu11 103.45(9) 3_455 3_455
Eu11 Ga17 Eu11 152.49(11) 4 3_455
As22 Ga18 As22 103.03(17) 3_455 4
As22 Ga18 As4 106.07(8) 3_455 2_565
As22 Ga18 As4 114.30(7) 4 2_565
As22 Ga18 As4 114.30(7) 3_455 1_565
As22 Ga18 As4 106.07(8) 4 1_565
As4 Ga18 As4 112.84(17) 2_565 1_565
As22 Ga18 Eu1 59.39(6) 3_455 6_565
As22 Ga18 Eu1 101.94(9) 4 6_565
As4 Ga18 Eu1 143.50(8) 2_565 6_565
As4 Ga18 Eu1 57.64(5) 1_565 6_565
As22 Ga18 Eu1 101.94(9) 3_455 5_566
As22 Ga18 Eu1 59.39(6) 4 5_566
As4 Ga18 Eu1 57.64(5) 2_565 5_566
As4 Ga18 Eu1 143.50(8) 1_565 5_566
Eu1 Ga18 Eu1 151.90(11) 6_565 5_566
Ga2 As1 Ga15 109.20(11) 2 7
Ga2 As1 Ga5 105.75(11) 2 .
Ga15 As1 Ga5 108.58(11) 7 .
Ga2 As1 Eu11 160.77(10) 2 7
Ga15 As1 Eu11 80.98(8) 7 7
Ga5 As1 Eu11 85.39(8) . 7
Ga2 As1 Eu12 85.08(8) 2 7
Ga15 As1 Eu12 81.13(8) 7 7
Ga5 As1 Eu12 161.33(11) . 7
Eu11 As1 Eu12 80.36(6) 7 7
Ga2 As1 Eu11 82.13(8) 2 3_455
Ga15 As1 Eu11 161.15(11) 7 3_455
Ga5 As1 Eu11 81.54(8) . 3_455
Eu11 As1 Eu11 84.15(6) 7 3_455
Eu12 As1 Eu11 85.03(6) 7 3_455
Ga4 As2 Ga3 109.16(12) . 2
Ga4 As2 Ga1 105.00(11) . 2
Ga3 As2 Ga1 108.92(11) 2 2
Ga4 As2 Eu1 161.43(10) . 2
Ga3 As2 Eu1 80.91(8) 2 2
Ga1 As2 Eu1 85.47(8) 2 2
Ga4 As2 Eu8 85.35(8) . 7
Ga3 As2 Eu8 81.69(8) 2 7
Ga1 As2 Eu8 161.02(11) 2 7
Eu1 As2 Eu8 80.65(6) 2 7
Ga4 As2 Eu2 82.24(8) . .
Ga3 As2 Eu2 160.47(10) 2 .
Ga1 As2 Eu2 82.18(8) 2 .
Eu1 As2 Eu2 84.12(6) 2 .
Eu8 As2 Eu2 83.57(6) 7 .
Ga2 As3 Ga4 111.68(12) 2 .
Ga2 As3 Ga6 108.01(12) 2 .
Ga4 As3 Ga6 108.05(11) . .
Ga2 As3 Ga16 109.34(10) 2 .
Ga4 As3 Ga16 109.27(12) . .
Ga6 As3 Ga16 110.49(11) . .
Ga18 As4 Ga7 107.97(11) 1_545 .
Ga18 As4 Ga1 106.32(10) 1_545 2
Ga7 As4 Ga1 108.12(12) . 2
Ga18 As4 Eu1 78.90(8) 1_545 6
Ga7 As4 Eu1 160.80(11) . 6
Ga1 As4 Eu1 86.26(9) 2 6
Ga18 As4 Eu2 158.41(12) 1_545 .
Ga7 As4 Eu2 84.00(8) . .
Ga1 As4 Eu2 85.99(9) 2 .
Eu1 As4 Eu2 84.41(6) 6 .
Ga8 As5 Ga1 111.40(12) . .
Ga8 As5 Ga7 108.09(11) . .
Ga1 As5 Ga7 108.05(11) . .
Ga8 As5 Ga16 109.07(12) . .
Ga1 As5 Ga16 109.05(10) . .
Ga7 As5 Ga16 111.19(11) . .
Ga17 As6 Ga6 107.41(10) . .
Ga17 As6 Ga2 106.05(10) . .
Ga6 As6 Ga2 108.09(11) . .
Ga17 As6 Eu3 158.97(12) . .
Ga6 As6 Eu3 84.36(8) . .
Ga2 As6 Eu3 85.89(9) . .
Ga17 As6 Eu11 80.23(8) . 4
Ga6 As6 Eu11 161.07(11) . 4
Ga2 As6 Eu11 85.55(9) . 4
Eu3 As6 Eu11 83.60(6) . 4
Ga9 As7 Ga1 107.65(11) . .
Ga9 As7 Ga14 107.28(11) . 4_545
Ga1 As7 Ga14 107.62(11) . 4_545
Ga9 As7 Eu2 80.80(8) . 6_556
Ga1 As7 Eu2 161.70(10) . 6_556
Ga14 As7 Eu2 84.38(8) 4_545 6_556
Ga9 As7 Eu1 162.31(11) . 5_556
Ga1 As7 Eu1 83.01(8) . 5_556
Ga14 As7 Eu1 81.87(9) 4_545 5_556
Eu2 As7 Eu1 85.18(6) 6_556 5_556
Ga9 As7 Eu1 81.07(8) . .
Ga1 As7 Eu1 84.09(8) . .
Ga14 As7 Eu1 161.99(11) 4_545 .
Eu2 As7 Eu1 81.22(6) 6_556 .
Eu1 As7 Eu1 86.18(6) 5_556 .
Ga2 As8 Ga3 109.22(11) . .
Ga2 As8 Ga8 104.99(11) . .
Ga3 As8 Ga8 108.69(11) . .
Ga2 As8 Eu5 161.63(11) . 7_556
Ga3 As8 Eu5 81.07(8) . 7_556
Ga8 As8 Eu5 85.09(8) . 7_556
Ga2 As8 Eu12 85.65(8) . 8_456
Ga3 As8 Eu12 81.51(8) . 8_456
Ga8 As8 Eu12 161.13(10) . 8_456
Eu5 As8 Eu12 80.80(6) 7_556 8_456
Ga2 As8 Eu3 82.27(8) . .
Ga3 As8 Eu3 160.60(11) . .
Ga8 As8 Eu3 82.17(8) . .
Eu5 As8 Eu3 84.00(6) 7_556 .
Eu12 As8 Eu3 83.93(6) 8_456 .
Ga3 As9 Ga9 108.49(12) . .
Ga3 As9 Eu9 85.42(10) . 7_556
Ga9 As9 Eu9 165.53(13) . 7_556
Ga3 As9 Eu1 82.46(9) . .
Ga9 As9 Eu1 83.42(9) . .
Eu9 As9 Eu1 102.85(16) 7_556 .
Ga3 As9 Eu5 82.61(9) . 7_556
Ga9 As9 Eu5 83.27(9) . 7_556
Eu9 As9 Eu5 94.94(16) 7_556 7_556
Eu1 As9 Eu5 155.70(9) . 7_556
Ga3 As9 Eu7 163.79(11) . 7_556
Ga9 As9 Eu7 87.72(9) . 7_556
Eu9 As9 Eu7 78.40(8) 7_556 7_556
Eu1 As9 Eu7 100.05(7) . 7_556
Eu5 As9 Eu7 99.64(7) 7_556 7_556
Ga13 As10 Ga5 106.59(11) 7 .
Ga13 As10 Ga12 107.69(11) 7 4
Ga5 As10 Ga12 109.74(11) . 4
Ga13 As10 Eu3 80.54(8) 7 6_565
Ga5 As10 Eu3 161.40(10) . 6_565
Ga12 As10 Eu3 83.44(8) 4 6_565
Ga13 As10 Eu12 161.20(11) 7 3_455
Ga5 As10 Eu12 83.67(8) . 3_455
Ga12 As10 Eu12 82.57(8) 4 3_455
Eu3 As10 Eu12 85.19(6) 6_565 3_455
Ga13 As10 Eu11 80.46(8) 7 7
Ga5 As10 Eu11 83.93(8) . 7
Ga12 As10 Eu11 160.38(11) 4 7
Eu3 As10 Eu11 80.32(6) 6_565 7
Eu12 As10 Eu11 85.16(6) 3_455 7
Ga4 As11 Ga15 109.01(11) . 7
Ga4 As11 Ga10 106.03(11) . .
Ga15 As11 Ga10 108.23(12) 7 .
Ga4 As11 Eu4 160.61(11) . 7
Ga15 As11 Eu4 80.59(8) 7 7
Ga10 As11 Eu4 85.93(8) . 7
Ga4 As11 Eu8 84.77(9) . 7
Ga15 As11 Eu8 81.19(9) 7 7
Ga10 As11 Eu8 161.65(10) . 7
Eu4 As11 Eu8 80.04(6) 7 7
Ga4 As11 Eu4 82.14(8) . .
Ga15 As11 Eu4 161.17(11) 7 .
Ga10 As11 Eu4 82.03(8) . .
Eu4 As11 Eu4 84.56(6) 7 .
Eu8 As11 Eu4 84.91(6) 7 .
Ga11 As12 Ga7 107.62(11) . .
Ga11 As12 Ga4 106.18(11) . .
Ga7 As12 Ga4 108.50(11) . .
Ga11 As12 Eu2 158.45(10) . .
Ga7 As12 Eu2 84.29(8) . .
Ga4 As12 Eu2 86.05(9) . .
Ga11 As12 Eu4 79.70(8) . .
Ga7 As12 Eu4 160.55(11) . .
Ga4 As12 Eu4 85.85(9) . .
Eu2 As12 Eu4 83.68(6) . .
Ga6 As13 Ga10 104.35(11) . .
Ga6 As13 Ga5 104.49(11) . .
Ga10 As13 Ga5 106.13(12) . .
Ga6 As13 Eu7 106.71(9) . .
Ga10 As13 Eu7 79.16(8) . .
Ga5 As13 Eu7 145.88(10) . .
Ga6 As13 Eu6 106.83(9) . 4
Ga10 As13 Eu6 145.90(10) . 4
Ga5 As13 Eu6 79.08(8) . 4
Eu7 As13 Eu6 78.99(6) . 4
Ga6 As14 Ga11 107.88(11) . .
Ga6 As14 Ga8 108.00(11) . .
Ga11 As14 Ga8 106.19(11) . .
Ga6 As14 Eu5 161.16(11) . .
Ga11 As14 Eu5 79.23(8) . .
Ga8 As14 Eu5 85.88(9) . .
Ga6 As14 Eu3 84.19(8) . .
Ga11 As14 Eu3 158.69(11) . .
Ga8 As14 Eu3 85.76(9) . .
Eu5 As14 Eu3 84.22(6) . .
Ga7 As15 Ga12 104.24(12) . .
Ga7 As15 Ga14 103.87(11) . 4_545
Ga12 As15 Ga14 107.76(12) . 4_545
Ga7 As15 Eu7 107.44(10) . 4_545
Ga12 As15 Eu7 145.31(10) . 4_545
Ga14 As15 Eu7 78.01(9) 4_545 4_545
Ga7 As15 Eu6 107.66(9) . .
Ga12 As15 Eu6 78.14(8) . .
Ga14 As15 Eu6 145.33(11) 4_545 .
Eu7 As15 Eu6 79.12(6) 4_545 .
Ga9 As16 Ga8 107.56(11) . .
Ga9 As16 Ga12 107.71(11) . .
Ga8 As16 Ga12 107.73(11) . .
Ga9 As16 Eu3 80.90(8) . 7_556
Ga8 As16 Eu3 161.60(11) . 7_556
Ga12 As16 Eu3 84.27(8) . 7_556
Ga9 As16 Eu5 162.20(11) . .
Ga8 As16 Eu5 82.99(8) . .
Ga12 As16 Eu5 81.61(8) . .
Eu3 As16 Eu5 85.11(6) 7_556 .
Ga9 As16 Eu5 81.19(8) . 7_556
Ga8 As16 Eu5 83.97(8) . 7_556
Ga12 As16 Eu5 161.55(10) . 7_556
Eu3 As16 Eu5 81.21(6) 7_556 7_556
Eu5 As16 Eu5 85.85(6) . 7_556
Ga9 As17 Ga13 106.73(11) . 6_556
Ga9 As17 Eu3 81.69(9) . 7_556
Ga13 As17 Eu3 81.61(8) 6_556 7_556
Ga9 As17 Eu2 81.49(8) . 6_556
Ga13 As17 Eu2 81.69(9) 6_556 6_556
Eu3 As17 Eu2 151.73(9) 7_556 6_556
Ga9 As17 Eu7 86.18(9) . 7_556
Ga13 As17 Eu7 167.10(11) 6_556 7_556
Eu3 As17 Eu7 100.57(7) 7_556 7_556
Eu2 As17 Eu7 100.80(7) 6_556 7_556
Ga9 As17 Eu6 166.60(11) . 6_556
Ga13 As17 Eu6 86.68(9) 6_556 6_556
Eu3 As17 Eu6 100.75(7) 7_556 6_556
Eu2 As17 Eu6 100.88(7) 6_556 6_556
Eu7 As17 Eu6 80.42(6) 7_556 6_556
Ga13 As18 Ga10 106.55(11) 7 .
Ga13 As18 Ga14 107.49(12) 7 .
Ga10 As18 Ga14 109.34(11) . .
Ga13 As18 Eu2 80.79(8) 7 7
Ga10 As18 Eu2 161.58(11) . 7
Ga14 As18 Eu2 83.58(8) . 7
Ga13 As18 Eu8 161.20(11) 7 .
Ga10 As18 Eu8 83.82(8) . .
Ga14 As18 Eu8 82.81(8) . .
Eu2 As18 Eu8 84.92(6) 7 .
Ga13 As18 Eu4 80.64(8) 7 7
Ga10 As18 Eu4 84.24(8) . 7
Ga14 As18 Eu4 160.54(10) . 7
Eu2 As18 Eu4 80.29(6) 7 7
Eu8 As18 Eu4 84.97(6) . 7
Ga11 As19 Ga10 105.51(11) . .
Ga11 As19 Eu8 155.70(11) . .
Ga10 As19 Eu8 86.06(9) . .
Ga11 As19 Eu4 78.42(8) . .
Ga10 As19 Eu4 84.21(9) . .
Eu8 As19 Eu4 81.68(6) . .
Ga11 As19 Eu9 102.18(15) . .
Ga10 As19 Eu9 145.87(16) . .
Eu8 As19 Eu9 76.45(11) . .
Eu4 As19 Eu9 121.02(11) . .
Ga11 As19 Eu7 105.07(10) . .
Ga10 As19 Eu7 78.48(9) . .
Eu8 As19 Eu7 98.09(7) . .
Eu4 As19 Eu7 162.65(9) . .
Eu9 As19 Eu7 75.34(10) . .
Ga11 As20 Ga12 103.91(11) . .
Ga11 As20 Eu12 156.52(11) . 2_655
Ga12 As20 Eu12 84.58(9) . 2_655
Ga11 As20 Eu5 77.76(8) . .
Ga12 As20 Eu5 82.62(9) . .
Eu12 As20 Eu5 81.78(6) 2_655 .
Ga11 As20 Eu6 105.67(10) . .
Ga12 As20 Eu6 77.80(8) . .
Eu12 As20 Eu6 97.47(7) 2_655 .
Eu5 As20 Eu6 160.37(9) . .
Ga11 As20 Eu10 110.72(15) . .
Ga12 As20 Eu10 138.59(16) . .
Eu12 As20 Eu10 72.67(11) 2_655 .
Eu5 As20 Eu10 125.90(12) . .
Eu6 As20 Eu10 71.64(11) . .
Ga15 As21 Ga13 108.14(11) . .
Ga15 As21 Eu10 85.24(11) . .
Ga13 As21 Eu10 165.59(14) . .
Ga15 As21 Eu4 82.27(9) . .
Ga13 As21 Eu4 83.12(9) . .
Eu10 As21 Eu4 104.5(2) . .
Ga15 As21 Eu11 82.56(8) . .
Ga13 As21 Eu11 82.72(9) . .
Eu10 As21 Eu11 94.1(2) . .
Eu4 As21 Eu11 154.87(9) . .
Ga15 As21 Eu6 162.98(11) . .
Ga13 As21 Eu6 88.88(9) . .
Eu10 As21 Eu6 77.82(9) . .
Eu4 As21 Eu6 100.24(7) . .
Eu11 As21 Eu6 100.13(7) . .
Ga18 As22 Ga14 104.42(12) 3_545 .
Ga18 As22 Eu8 155.75(10) 3_545 .
Ga14 As22 Eu8 84.72(9) . .
Ga18 As22 Eu1 77.47(6) 3_545 8
Ga14 As22 Eu1 83.21(9) . 8
Eu8 As22 Eu1 81.47(6) . 8
Ga18 As22 Eu7 106.09(8) 3_545 .
Ga14 As22 Eu7 77.50(8) . .
Eu8 As22 Eu7 97.76(7) . .
Eu1 As22 Eu7 160.68(9) 8 .
Ga18 As22 Eu9 109.55(13) 3_545 .
Ga14 As22 Eu9 139.60(14) . .
Eu8 As22 Eu9 73.20(9) . .
Eu1 As22 Eu9 124.73(10) 8 .
Eu7 As22 Eu9 72.65(9) . .
Ga17 As23 Ga5 105.23(12) 3_545 4_545
Ga17 As23 Eu12 156.47(10) 3_545 2_655
Ga5 As23 Eu12 85.89(9) 4_545 2_655
Ga17 As23 Eu10 101.40(18) 3_545 .
Ga5 As23 Eu10 146.88(19) 4_545 .
Eu12 As23 Eu10 77.09(14) 2_655 .
Ga17 As23 Eu11 78.94(6) 3_545 2_655
Ga5 As23 Eu11 83.48(9) 4_545 2_655
Eu12 As23 Eu11 81.90(6) 2_655 2_655
Eu10 As23 Eu11 121.11(13) . 2_655
Ga17 As23 Eu6 104.86(8) 3_545 .
Ga5 As23 Eu6 78.89(8) 4_545 .
Eu12 As23 Eu6 97.53(7) 2_655 .
Eu10 As23 Eu6 75.51(13) . .
Eu11 As23 Eu6 162.35(9) 2_655 .
Ga15 As24 Ga3 102.55(11) . 8
Ga15 As24 Eu10 83.60(11) . .
Ga3 As24 Eu10 171.47(18) 8 .
Ga15 As24 Eu9 173.44(15) . 2_655
Ga3 As24 Eu9 82.32(10) 8 2_655
Eu10 As24 Eu9 91.13(11) . 2_655
Ga15 As24 Eu8 80.40(8) . .
Ga3 As24 Eu8 80.44(8) 8 .
Eu10 As24 Eu8 106.6(2) . .
Eu9 As24 Eu8 104.94(15) 2_655 .
Ga15 As24 Eu12 80.20(8) . .
Ga3 As24 Eu12 80.20(8) 8 .
Eu10 As24 Eu12 95.2(2) . .
Eu9 As24 Eu12 96.46(15) 2_655 .
Eu8 As24 Eu12 148.79(9) . .
Ga15 As24 Eu9 117.35(14) . .
Ga3 As24 Eu9 122.56(15) 8 .
Eu10 As24 Eu9 57.84(19) . .
Eu9 As24 Eu9 62.3(2) 2_655 .
Eu8 As24 Eu9 68.43(7) . .
Eu12 As24 Eu9 142.71(9) . .
Ga15 As24 Eu10 116.01(17) . 2_655
Ga3 As24 Eu10 123.44(17) 8 2_655
Eu10 As24 Eu10 48.0(3) . 2_655
Eu9 As24 Eu10 57.43(18) 2_655 2_655
Eu8 As24 Eu10 142.77(10) . 2_655
Eu12 As24 Eu10 68.30(8) . 2_655
Eu9 As24 Eu10 74.41(9) . 2_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Eu1 As4 3.020(2) 6_556
Eu1 As9 3.043(3) .
Eu1 As22 3.093(3) 8_456
Eu1 As2 3.102(2) 2
Eu1 As7 3.154(2) 5_556
Eu1 As7 3.174(2) .
Eu1 Ga18 3.5081(14) 5_566
Eu1 Ga3 3.665(3) .
Eu1 Ga9 3.716(3) .
Eu1 Ga14 3.744(3) 8_456
Eu1 Eu8 4.0161(16) 8_456
Eu1 Eu2 4.0711(16) 6_556
Eu2 As17 3.022(3) 6
Eu2 As12 3.033(2) .
Eu2 As4 3.041(2) .
Eu2 As7 3.080(2) 6
Eu2 As18 3.094(2) 7
Eu2 As2 3.195(2) .
Eu2 Ga9 3.636(3) 6
Eu2 Ga13 3.644(3) .
Eu2 Ga7 3.711(3) .
Eu2 Eu4 4.0459(16) .
Eu2 Eu8 4.1977(16) 7
Eu3 As17 3.017(2) 7_556
Eu3 As6 3.028(2) .
Eu3 As14 3.037(2) .
Eu3 As16 3.078(2) 7_556
Eu3 As10 3.093(2) 6_566
Eu3 As8 3.184(2) .
Eu3 Ga13 3.637(3) 4
Eu3 Ga9 3.639(3) 7_556
Eu3 Ga6 3.710(3) .
Eu3 Eu11 4.0380(16) 4
Eu3 Eu5 4.0623(16) .
Eu3 Eu12 4.2047(16) 8_456
Eu4 As12 3.033(2) .
Eu4 As21 3.041(3) .
Eu4 As19 3.091(3) .
Eu4 As11 3.111(2) 7
Eu4 As18 3.180(2) 7
Eu4 As11 3.185(2) .
Eu4 Ga11 3.544(3) .
Eu4 Ga15 3.659(3) .
Eu4 Ga13 3.703(3) .
Eu4 Eu8 4.0098(16) .
Eu4 Eu4 4.236(2) 7
Eu5 As14 3.021(2) .
Eu5 As9 3.046(3) 7_556
Eu5 As20 3.095(3) .
Eu5 As8 3.102(2) 7_556
Eu5 As16 3.142(2) .
Eu5 As16 3.163(2) 7_556
Eu5 Ga11 3.522(3) .
Eu5 Ga3 3.672(3) 7_556
Eu5 Ga9 3.713(3) 7_556
Eu5 Ga12 3.724(3) .
Eu5 Eu12 4.0216(16) 2_655
Eu6 As21 3.092(2) .
Eu6 As17 3.184(3) 6
Eu6 As20 3.204(3) .
Eu6 As23 3.209(3) .
Eu6 As15 3.225(2) .
Eu6 As13 3.235(3) 4_545
Eu6 Ga12 3.627(3) .
Eu6 Ga5 3.664(3) 4_545
Eu6 Eu10 3.838(4) .
Eu6 Eu7 4.1053(18) 4_545
Eu7 As9 3.110(3) 7_556
Eu7 As17 3.175(3) 7_556
Eu7 As22 3.212(3) .
Eu7 As19 3.216(3) .
Eu7 As13 3.220(3) .
Eu7 As15 3.221(3) 4
Eu7 Ga14 3.622(3) .
Eu7 Ga10 3.655(3) .
Eu7 Eu9 3.856(3) .
Eu8 As19 3.041(2) .
Eu8 As22 3.061(3) .
Eu8 As2 3.104(2) 7
Eu8 As24 3.116(3) .
Eu8 As11 3.124(3) 7
Eu8 As18 3.124(2) .
Eu8 Ga15 3.691(3) .
Eu8 Ga3 3.695(3) 8
Eu8 Eu9 3.795(3) .
Eu9 As9 2.989(4) 7_556
Eu9 As24 3.068(4) 2_655
Eu9 As19 3.092(5) .
Eu9 Eu10 3.243(10) .
Eu9 As22 3.296(6) .
Eu9 Eu9 3.476(11) 2_655
Eu9 As24 3.595(4) .
Eu9 Ga3 3.729(4) 7_556
Eu9 Eu10 4.357(5) 2_655
Eu10 Eu10 2.755(15) 2_655
Eu10 As21 3.019(5) .
Eu10 As24 3.033(4) .
Eu10 As23 3.057(7) .
Eu10 As20 3.351(8) .
Eu10 As24 3.609(5) 2_655
Eu10 Ga15 3.748(4) .
Eu10 Eu12 3.800(4) 2_655
Eu10 Eu11 4.434(7) .
Eu11 As6 3.030(2) 4_545
Eu11 As21 3.041(2) .
Eu11 As23 3.093(3) 2_655
Eu11 As1 3.108(2) 7
Eu11 As10 3.168(2) 7
Eu11 As1 3.172(2) 3_545
Eu11 Ga17 3.5625(14) 3_545
Eu11 Ga15 3.670(3) .
Eu11 Ga13 3.689(3) .
Eu11 Ga5 3.745(3) 3_545
Eu11 Ga2 3.759(3) 4_545
Eu11 Eu12 4.0203(16) .
Eu12 As23 3.041(2) 2_655
Eu12 As20 3.049(3) 2_655
Eu12 As8 3.103(2) 8
Eu12 As10 3.119(2) 3_545
Eu12 As24 3.121(3) .
Eu12 As1 3.123(2) 7
Eu12 Ga15 3.687(3) .
Eu12 Ga3 3.689(3) 8
Eu12 Ga12 3.759(3) 2_655
Ga1 As5 2.421(3) .
Ga1 As4 2.473(3) 2
Ga1 As7 2.496(3) .
Ga1 As2 2.506(3) 2
Ga2 As3 2.420(3) 2
Ga2 As6 2.472(3) .
Ga2 As8 2.490(3) .
Ga2 As1 2.498(3) 2
Ga3 As9 2.480(3) .
Ga3 As2 2.502(3) 2
Ga3 As8 2.505(3) .
Ga3 As24 2.569(3) 8_456
Ga4 As3 2.425(3) .
Ga4 As12 2.471(3) .
Ga4 As2 2.492(3) .
Ga4 As11 2.501(3) .
Ga5 As13 2.439(3) .
Ga5 As23 2.491(3) 4
Ga5 As1 2.511(3) .
Ga5 As10 2.524(3) .
Ga6 As3 2.427(3) .
Ga6 As13 2.429(3) .
Ga6 As14 2.461(3) .
Ga6 As6 2.462(3) .
Ga7 As5 2.427(3) .
Ga7 As15 2.428(3) .
Ga7 As12 2.461(3) .
Ga7 As4 2.468(3) .
Ga8 As5 2.419(3) .
Ga8 As14 2.477(3) .
Ga8 As16 2.495(3) .
Ga8 As8 2.506(3) .
Ga9 As7 2.488(3) .
Ga9 As16 2.489(3) .
Ga9 As9 2.511(3) .
Ga9 As17 2.518(3) .
Ga10 As13 2.438(3) .
Ga10 As19 2.494(3) .
Ga10 As11 2.508(3) .
Ga10 As18 2.522(3) .
Ga11 As12 2.454(3) .
Ga11 As20 2.461(3) .
Ga11 As14 2.462(3) .
Ga11 As19 2.462(3) .
Ga12 As15 2.448(3) .
Ga12 As20 2.506(3) .
Ga12 As16 2.508(3) .
Ga12 As10 2.540(3) 4_545
Ga13 As18 2.483(3) 7
Ga13 As10 2.488(3) 7
Ga13 As21 2.509(3) .
Ga13 As17 2.519(3) 6
Ga14 As15 2.456(3) 4
Ga14 As22 2.506(3) .
Ga14 As7 2.512(3) 4
Ga14 As18 2.543(3) .
Ga15 As21 2.486(3) .
Ga15 As1 2.500(3) 7
Ga15 As11 2.501(3) 7
Ga15 As24 2.566(3) .
Ga16 As3 2.429(3) 2
Ga16 As3 2.429(3) .
Ga16 As5 2.429(3) .
Ga16 As5 2.429(3) 2
Ga17 As6 2.456(3) 2
Ga17 As6 2.456(3) .
Ga17 As23 2.457(3) 4
Ga17 As23 2.457(3) 3_455
Ga18 As22 2.457(3) 3_455
Ga18 As22 2.457(3) 4
Ga18 As4 2.459(3) 2_565
Ga18 As4 2.459(3) 1_565
